# II. Types of Magnetism

of 11
/11

Embed Size (px)

### Transcript of II. Types of Magnetism

1(1) Diamagnetism:

(2) Paramagnetism:

(3) Ferromagnetism:

(4) Antiferromagnetism:

(5) Ferrimagnetism:

II. Types of Magnetism

Current, i = = =

An additional postulate, mυr = n(h/2π) (quantized angular momentum)

orbital motion → electronic moment

Orbit motion : Bohr model

v

spectrum under a magnetic field :

Anomalous Zeeman Effect

μspin =

→ A fundamental quantity called,

(1) Diamagnetism

No net atomic moment : μr < 1, χ < 0

Classical theory, 1905 yr Paul Langevin (see Cullity)

For an e_ in orbital motion, no net μorbit of paired electrons if Ha = 0,

A net μorbit within atom opposing the flux change(Lentz law) due to accelerated or decelerated orbital motion

of e_ if Ha > 0.

On the basis of Bohr model, μorbit = = since = – erH/2mc

If H is not perpendicular to the orbit plane, μorbit =

For an atom with Z outer electrons, μorbit =

For a bulk magnetization, where, No = Abogadro's number, ρ = density, and W = atomic number : independent of temperature!

Diamagnetism in superconductors

- For H < Hc in type I superconductors and H < Hc1 in

type II superconductors,

Origin: shielding supercurrent in the case of zero-field-cooling

Meissner effect in the case of field-cooling

- For Hc1 < H < Hc2 in type II superconductors,

mixed (or vortex) state : B > 0

c

er

Classical theory, Lamor frequency L

The torque causes the orientation of the angular momentum vector L (and thus the orbital magnetic dipole moment orb) to change by dL perpendicular to both B and orbit. (see Fig. 3.3 in O’Handley)

Since dL = Lsind = LLsindt, and the torque dL/dt = orbitBsin as = dL/dt = orbitB

Therefore, L = orbitB/L = oB = eB/2m

An angular rotation of the orbital magnetic moment vector orbit with L // B

An electric current i equivalent to the Lamor precession of an orbit electron

i = (charge)(revolution per unit time) = (– e)/(L/2) = – e2B/4m

Thus, μorbit = iA = (– e2B/4m)(r2) = – (e2r2/4m)B

For the Lamor precession of Z electrons

μorbit = – Ze2B<r2>/4m

μorbit = – Ze2B<r2>/6m

where, Nv = number of atoms per unit volume

(1) Diamagnetism (additional)

μr > 1, χ > 0

Experimental

Cuire law

χ =

Langevin theory

m = mo + ms

Assuming all m are identical and non-interacting,

and m depends on H and thermal agitation,

According to classical Boltzman statistics,

Probability having E, P(E)

= exp

1

L(a)

a

Magnetization, M = NmL(a), where

Let Nm = Mo (maximum possible magnetization,

corresponding to the perfect alignment of all m parallel to H:

a state of complete saturation)

Then ,

Weiss theory

an interacting field He (called, molecular field or

exchange field)

Htot = H + He

→ leading to Curie-Weiss law

(2) Paramagnetism (continued)

Remember the following;

where, |J| =

In general, Lande equation

If L = 0, J = S → g = 2 (only spin contribution)

If S = 0, J = L → g = 1 (only orbital contribution)

If J = ∞ : random orientation (classical)

T

C

H

M

tot

(2) Paramagnetism (continued)

Localized electron model

Magnetic potential energy,

E = μtotal • B (μtotal : total magnetic moment of an atom or net atomic magnetic moment)

= gμB(J/) • B (|J| = , : total angular momentum)

= gμB(Jz/)B

= gμBMJB since Jz = MJ (MJ : total magnetic quantum number)

where, MJ can have only 2J + 1 values

MJ = -J, -(J-1), ..., (J-1), J (J : total angular momentum quantum number)

Therefore, the average magnetization in B is given by

Applying Boltzman statistics, Nv = N/V,

M = NvgμB where

BJ(x) is Brilliouin function If J = ∞ → BJ(x) = L(a) : classical distribition

If J = : one spin /atom, = tanhx

kT

(2) Paramagnetism (continued)

Comments

Comparison of quantum picture with classical one Brillouin function vs Lagevin fun

(see Fig. 3.15 in O’Handley) (see Fig. 3.16 in O’Handley)

Electronic Materials & Devices Laboratory Seoul National University Department of Material Science & Engineering

Example (see Fig. 3.17 in O’Handley)

(2) Paramagnetism (continued)

(2) Paramagnetism (continued)

Pauli Paramagnetism (examples: see Fig. 11 in Chap. 4 of Kittel)

- Conduction electron paramagnetism for indistinguishable free electron spins in a metal

- Only Fermi particles within ±kT/2 of Fermi energy EF can change their energy(i.e., orientation) in

response to an allpiled field.

- As T increases, more carriers are excited above the Fermi level and excited carriers are able to be

aligned by the field.

For free electrons in weak fields, x(μmB/kT)1 in localized electron theory, the susceptibility χPauli

χPauli ≈ = : independent of T

More precisely, by considering the spin imbalance in two free electron bands subject to a weak Zeeman

splitting ( μmBEF) :

Temperature independence of χPauli : with increasing temperature, increased free electron spins able to

align with an external field and increased thermal disordering of those aligned spins are cancelled.

FE

kT

kT

(2) Paramagnetism (continued)

(2) Paramagnetism:

(3) Ferromagnetism:

(4) Antiferromagnetism:

(5) Ferrimagnetism:

II. Types of Magnetism

Current, i = = =

An additional postulate, mυr = n(h/2π) (quantized angular momentum)

orbital motion → electronic moment

Orbit motion : Bohr model

v

spectrum under a magnetic field :

Anomalous Zeeman Effect

μspin =

→ A fundamental quantity called,

(1) Diamagnetism

No net atomic moment : μr < 1, χ < 0

Classical theory, 1905 yr Paul Langevin (see Cullity)

For an e_ in orbital motion, no net μorbit of paired electrons if Ha = 0,

A net μorbit within atom opposing the flux change(Lentz law) due to accelerated or decelerated orbital motion

of e_ if Ha > 0.

On the basis of Bohr model, μorbit = = since = – erH/2mc

If H is not perpendicular to the orbit plane, μorbit =

For an atom with Z outer electrons, μorbit =

For a bulk magnetization, where, No = Abogadro's number, ρ = density, and W = atomic number : independent of temperature!

Diamagnetism in superconductors

- For H < Hc in type I superconductors and H < Hc1 in

type II superconductors,

Origin: shielding supercurrent in the case of zero-field-cooling

Meissner effect in the case of field-cooling

- For Hc1 < H < Hc2 in type II superconductors,

mixed (or vortex) state : B > 0

c

er

Classical theory, Lamor frequency L

The torque causes the orientation of the angular momentum vector L (and thus the orbital magnetic dipole moment orb) to change by dL perpendicular to both B and orbit. (see Fig. 3.3 in O’Handley)

Since dL = Lsind = LLsindt, and the torque dL/dt = orbitBsin as = dL/dt = orbitB

Therefore, L = orbitB/L = oB = eB/2m

An angular rotation of the orbital magnetic moment vector orbit with L // B

An electric current i equivalent to the Lamor precession of an orbit electron

i = (charge)(revolution per unit time) = (– e)/(L/2) = – e2B/4m

Thus, μorbit = iA = (– e2B/4m)(r2) = – (e2r2/4m)B

For the Lamor precession of Z electrons

μorbit = – Ze2B<r2>/4m

μorbit = – Ze2B<r2>/6m

where, Nv = number of atoms per unit volume

(1) Diamagnetism (additional)

μr > 1, χ > 0

Experimental

Cuire law

χ =

Langevin theory

m = mo + ms

Assuming all m are identical and non-interacting,

and m depends on H and thermal agitation,

According to classical Boltzman statistics,

Probability having E, P(E)

= exp

1

L(a)

a

Magnetization, M = NmL(a), where

Let Nm = Mo (maximum possible magnetization,

corresponding to the perfect alignment of all m parallel to H:

a state of complete saturation)

Then ,

Weiss theory

an interacting field He (called, molecular field or

exchange field)

Htot = H + He

→ leading to Curie-Weiss law

(2) Paramagnetism (continued)

Remember the following;

where, |J| =

In general, Lande equation

If L = 0, J = S → g = 2 (only spin contribution)

If S = 0, J = L → g = 1 (only orbital contribution)

If J = ∞ : random orientation (classical)

T

C

H

M

tot

(2) Paramagnetism (continued)

Localized electron model

Magnetic potential energy,

E = μtotal • B (μtotal : total magnetic moment of an atom or net atomic magnetic moment)

= gμB(J/) • B (|J| = , : total angular momentum)

= gμB(Jz/)B

= gμBMJB since Jz = MJ (MJ : total magnetic quantum number)

where, MJ can have only 2J + 1 values

MJ = -J, -(J-1), ..., (J-1), J (J : total angular momentum quantum number)

Therefore, the average magnetization in B is given by

Applying Boltzman statistics, Nv = N/V,

M = NvgμB where

BJ(x) is Brilliouin function If J = ∞ → BJ(x) = L(a) : classical distribition

If J = : one spin /atom, = tanhx

kT

(2) Paramagnetism (continued)

Comments

Comparison of quantum picture with classical one Brillouin function vs Lagevin fun

(see Fig. 3.15 in O’Handley) (see Fig. 3.16 in O’Handley)

Electronic Materials & Devices Laboratory Seoul National University Department of Material Science & Engineering

Example (see Fig. 3.17 in O’Handley)

(2) Paramagnetism (continued)

(2) Paramagnetism (continued)

Pauli Paramagnetism (examples: see Fig. 11 in Chap. 4 of Kittel)

- Conduction electron paramagnetism for indistinguishable free electron spins in a metal

- Only Fermi particles within ±kT/2 of Fermi energy EF can change their energy(i.e., orientation) in

response to an allpiled field.

- As T increases, more carriers are excited above the Fermi level and excited carriers are able to be

aligned by the field.

For free electrons in weak fields, x(μmB/kT)1 in localized electron theory, the susceptibility χPauli

χPauli ≈ = : independent of T

More precisely, by considering the spin imbalance in two free electron bands subject to a weak Zeeman

splitting ( μmBEF) :

Temperature independence of χPauli : with increasing temperature, increased free electron spins able to

align with an external field and increased thermal disordering of those aligned spins are cancelled.

FE

kT

kT

(2) Paramagnetism (continued)